Luminescence behavior of silicon and carbon nanoparticles dispersed in low-polar liquids
© Ryabchikov et al.; licensee Springer. 2012
Received: 30 April 2012
Accepted: 12 June 2012
Published: 2 July 2012
A comparative photoluminescence analysis of as-prepared and chemically modified (by alkyl chains -C18H37) silicon and carbon nanoparticles dispersed in low-polar liquids is reported. Influence of the low-polar liquid nature and ambient temperature on photoluminescence of the nanoparticles has been investigated from the point of view of their possible application as thermal nanoprobes.
Low-dimensional structures present considerable interest for researchers because of their new and unique optical and electronic properties in comparison with bulk materials. For example, various nanoparticles (NPs) are involved in different applications such as electronics , photovoltaic , biology , liquid crystals  etc. Photoluminescence (PL) is one of the important phenomena taking place in semiconductor NPs. It is very sensitive to various experimental conditions, such as molecular ambient environment, temperature, pressure, and so on. In particular, thermally induced PL effects are of special interest for temperature probing at nanoscale in various media. For example, different materials are reported to be used as thermal-sensitive nanoprobes  and nanothermometers .
A comparative analysis of the influence of high- and low-polar liquids (LPLs) on PL of Si NPs has already been reported . The low-polar liquids were reported to be used instead of the high-polar liquids in order to prevent PL quenching of the NPs. However, stable colloidal solutions of the as-prepared Si NPs could not be obtained in LPLs because of their oleophobic surface. Thus, surface chemical modification of the NPs by different alkyl groups can be the simplest way to overcome this problem .
In this work, we have studied the influence of LPLs, ambient temperature, and continuous laser irradiation on PL behavior of Si and C NPs in view of their temperature-sensing applications.
Chemical anodic etching of p-type 10-Ω·cm (100)-oriented Si wafer has been used for the preparation of nano-Si powder. Silicon substrate was etched in a solution containing 1:1 volume mixture of HF (48%) and anhydrous ethanol. Anodic current density was 45 mA/cm2, and etching time is 50 min. A permanent stirring of the etching solution was applied in order to evacuate hydrogen bubbles formed during the etching process. The anodization was performed in a Teflon cell with a copper electrode as a backside contact. The counter electrode was made of platinum. After the etching, a highly porous network constituted by numerous interconnected nanocrystals was formed. The sample was washed with anhydrous ethanol several times, dried in ambient air, and then scratched out from the wafer. Mechanical dry grinding of the formed free nanoporous layer transformed it into a powder state.
Thermal hydrosilylation approach, described in details in the review , was used for the grafting of alkyl groups (−C18H37) onto the surface of Si nanoparticles. Freshly prepared powder (30 mg) was treated with 1.5 mL of 1-octadecene at 150°C for 16 h under magnetic stirring in N2 atmosphere. The reaction mixture was cooled to room temperature and centrifuged for 10 min at 20,000 × g to remove large particles.
Photoluminescent C NPs with the surface substantially covered with carboxylic acid groups were prepared by means of electrochemical dissolution of SiC wafers. To functionalize their surface with -C18H37 groups, the powder of C NPs was refluxed for 1 h with the excess of octadecylamine C18H37NH2 in anhydrous o-xylene; according to FTIR data, the amide bonds are formed between C NPs and C18H37NH2. The liquid was then slowly distilled out (in the stream of N2, bath temperature did not exceed 155°C); afterwards, a small portion of o-xylene was added and distilled out to remove residues of H2O which form the reaction mixture. To workup alkylated carbon nanoparticles, residue after solvent evaporation was redispersed in n-hexane and extracted several times by 0.5 mol/L HCl in methanol to remove excess of C18H37NH2, then washed twice with H2O, centrifuged (20,000 × g, 2 × 10 min) to remove any products, insoluble in hexane, than the hexane solution allowed to evaporate and dried in air at 85°C. Brown waxy residue of alkylated C NPs is readily dispersible in non-polar solvents.
Photoluminescence excitation of all NPs was performed by means of argon-ion laser with excitation photon energy at 2.54 eV. The laser spot area was about 10−4 cm−2. Additionally, laser diode with the excitation photon energy at 3.62 eV has been used for the excitation of C-C18H37 NPs. All colloidal solutions of the NPs were put in a UV transparent quartz cuvette in a volume of 1 mL. Temperature dependence PL measurements were carried out using ViscoTerm VT100 temperature cell (VISCO Pump & Seal Group, Brooklyn, Victoria, Australia). In this case, the colloidal solutions were placed in a special sample holder. HORIBA Jobin Yvon (Edison, NJ, USA) iHR-320 monochromator was used for spectral decomposition of the PL signal. The PL spectra of the colloidal solutions were detected by nitrogen-cooled CCD camera HORIBA Symphony 1024 × 256 (HORIBA Jobin Yvon Edison, NJ, USA). All PL spectra were corrected using the spectral response function of the whole experimental setup.
Results and discussion
It is worth to note that the performed surface chemical modification by the same alkyl groups impacts differently surface states of the Si and C NPs and, consequently, their original PL spectra. As one can state, the red (110 meV) and blue (160 meV) shifts of the PL maxima occur for Si and C NPs, respectively. This fact can be explained by different influences of the grafted -C18H37 groups on density of the band tail electronic states (surface states) involved in radiative transitions of the charge carriers photogenerated in the studied NPs. In particular, the surface chemical modification by alkyl groups leads to increase of this state density for Si NPs and to its decrease for C NPs.
The observed PL changes of the NPs after their dispersion in the LPLs can be explained by reduction of the Förster resonant energy transfer (FRET) efficiency between NPs of different sizes. Indeed, the electronic interaction between the NPs in powder state in air is very strong because they are situated close to each other. It leads to higher FRET probability from small NPs with larger bandgaps toward big NPs having smaller bandgaps. Thus, the small NPs are optically inactive from photo-stimulated emission point of view. In contrast, they are more efficiently separated from each other after their dispersion in LPLs. Indeed, since the probability of the FRET event depends strongly on the distance D between two particles (approximately D−6), the resulting probability of the energy transfer in this case is dramatically reduced. Thus, the probability of the radiative recombination of the photoexcited charge carriers in the smaller NPs is considerably enhanced. Consequently, they become optically active and give their contribution in the PL spectrum resulting in the observed blue shift and broadening. Since no influence of the LPL nature on PL properties of the NPs dispersed in them was observed (see Figure 2 and corresponding discussion above), the FRET mechanism appears as the most preponderant.
Surface chemical modification of Si and C NPs by alkyl chains has succeeded. Perfectly stable and homogeneous colloidal solutions of these NPs in LPLs were obtained. Influence of LPLs, ambient temperature, and irradiation time on PL properties of the NPs was investigated. The linear temperature-dependent integrated PL intensity and spectral position paves the way for the application of this kind of colloidal solutions as temperature-sensitive media. Furthermore, the use of photoexciting power values under a critical threshold (for example, 10 mW for Si-C18H37 NPs dispersed in squalane) ensures necessary photostability of the colloidal solutions for temperature estimation applications.
YVR has obtained his M.S. degree in Solid State Physics in 1997 and his Ph.D. degree in the field of Semiconductor Nanostructures at M.V. Lomonosov Moscow State University in 2007. In 2008, he was invited at Helmholtz-Zentrum Berlin (HZB) in the framework of DAAD fellowship. In 2009, he was employed as a young scientific researcher at the P.N. Lebedev Physical Institute of Russian Academy of Sciences. Since 2012, he has a postdoctoral position at Lyon Institute of Nanotechnologies. His main scientific interest focuses on spectroscopic investigations based on silicon semiconductor nanostructures. VVL has received his M.S. degree in Semiconductor Physics and Electronics from Kiev National Shevchenko University in 1995 and his Ph.D. degree in the field of Integrated Electronic Devices from Ecole Centrale de Lyon (France) in 1998. He was employed as a scientific researcher by the French National Center of Scientific Researches in 2002. Currently, he works at Lyon Institute of Nanotechnologies in the Spectroscopies of Nanomaterials team. His main scientific interest is focused on elaboration, spectroscopic studies of physicochemical properties and multidisciplinary applications of nanomaterials of the IVth group. J-MB obtained his Ph.D. degree in 1996 at the University of Montpellier in the field of Condensed Matter. After two postdoctoral positions in Grenoble, he joined INSA of Lyon as an associate professor in 1999. Currently, he is conducting his research activities in the Lyon Institute of Nanotechnology. His main scientific activity focuses on spectroscopic characterizations of semiconductors nanostructures. SAA received his master's degree in Chemistry from Kiev National Taras Shevchenko University in 1998 and then his Ph.D. degree in Chemistry at the same university in 2003 for his work on the Immobilization of Organic Acids on Silica Gel Surface, Thermochemical and Catalytic Properties of Materials Obtained. Currently, SAA is working as an associate professor in the Chemistry Faculty of the same university. From 2004, SAA has close scientific collaboration with INSA Lyon (France); he participated in European projects such as INTAS, IRSES, and LST. Fields of his research interests are as follows: surface chemistry of nanostructured materials (semiconductors, inorganic oxides), surface functionalization and characterization, application of nanostructures in LDI mass-spectrometry, sensors, catalysis.
The authors acknowledge INSA-LYON for the financial support under the BQR 2011 project. One of us, Sergei Alekseev, also thanks INSA-LYON for the invitation as an associate professor. We are grateful to D Philippon and P Vergne from LaMCoS for the temperature cell Viscoterm VT100.
- Panthani MG, Korgel BA: Nanocrystals for electronics. Chem Biomol Eng 2012, 3: 287–311. 10.1146/annurev-chembioeng-062011-081040View ArticleGoogle Scholar
- Fu H, Tsang T-W: Infrared colloidal lead chalcogenide nanocrystals: synthesis, properties, and photovoltaic applications. Nanoscale 2012, 4: 2187–2201. 10.1039/c2nr11836jView ArticleGoogle Scholar
- Chamakura K, Perez-Ballestero R, Luo Z, Bashir S, Liu J: Comparison of bactericidal activities of silver nanoparticles with common chemical disinfectants. Colloids Surf B Biointerfaces 2011, 84(1):88–96. 10.1016/j.colsurfb.2010.12.020View ArticleGoogle Scholar
- Stamatoiu O, Mirzaei J, Feng X, Hegmann T: Nanoparticles in liquid crystals and liquid crystalline nanoparticles. Top Curr Chem 2012, 318: 331–393.View ArticleGoogle Scholar
- Chattopadhyay S, Sen P, Andrews JT, Sen PK: Semiconductor core-shell quantum dot: a low temperature nano-sensor material. J Appl Phys 2012, 111: 034310. 10.1063/1.3681309View ArticleGoogle Scholar
- Cui Y, Xu H, Yue Y, Guo Z, Yu J, Chen Z, Gao J, Yang Y, Qian G, Chen B: A luminescent mixed-lanthanide metal–organic framework thermometer. J Am Chem Soc 2012, 134(9):3979–3982. 10.1021/ja2108036View ArticleGoogle Scholar
- Fellah S, Wehrspohn RB, Gabouze N, Ozanam F, Chazalviel J-N: Photoluminescence quenching of porous silicon in organic solvents: evidence for dielectric effects. J Luminescence 1998, 80(1–4):109–113.View ArticleGoogle Scholar
- Huck LA, Buriak JM: Toward a mechanistic understanding of exciton-mediated hydrosilylation on nanocrystalline silicon. J Am Chem Soc 2012, 134(1):489–497. 10.1021/ja208604rView ArticleGoogle Scholar
- Buriak JM: Organometallic chemistry on silicon and germanium surfaces. Chem Rev 2002, 102(5):1271–1308. 10.1021/cr000064sView ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.